Preface Welding: The Permanent Bond Between Two Solid Bodies What a long story welding is! Seeing the light of day at the end of the 19thcentury in the mind of scientists, it passed quickly into the hands of technicians, firstof all with the oxyacetylene technique, then with arc welding and resistance weldingtechniques. Other processes (we will not quote them all in this introduction) thenfollowed and the 20th century ended with laser welding which had its origins in the1980s. However, it must be said that only since the 1950s has welding been the mainmeans of assembly, as riveting was the most used method up to that point. In fact, after abandoning this method to some extent, scientists renewed theirinvolvement in the 1930s. In France, at the time, Albert Portevin set out Les basesscientifiques de la soudure autogène and a higher education teaching programmebegan in 1931 at L’Institut de soudure. In the 1930s welding was implicated inbridge failures, notably in Germany and Belgium, then during World War II camethe failure of Liberty ships constructed in great numbers thanks to the technique ofwelding. Other later catastrophic failures affected pressure vessels. It is in thiscontext that in 1948 L’Institut international de la soudure (IIS/IIW) was founded. Itmet the need for international collaboration, in particular with regard to safety andresearch, expressed by different national bodies and by the whole welding world,from scientists to users. Today in 2008, the IIS/IIW holds its 61st annual meeting: 16commissions, with sub-commissions and study groups, cover the whole field ofwelding, from design to performance and safety, including teaching and research.This demonstrates the importance of this collaboration and the richness of itscontribution.
xiv Metallurgy and Mechanics of Welding Welding can be regarded, like the language of Aesop, as the best and worst ofthings. Indeed, it makes it possible to bond almost all materials, from metals toplastics, with continuity; however, this does not imply homogenity. The processesand hence possibilities are very numerous depending on the types of assemblies tobe made, the properties required and evident economic constraints to be respected.At the same time welding can be regarded as the weak link of the majority ofconstructions as it is often called into question when problems arise. In the examplescited above (bridges, Liberty ships, pressure vessels) it is the welding that is calledinto question each time – often it must be added linked to a parent metal whoseresistance to a sudden failure is insufficient. The phenomena that occur during welding are both numerous and complex. Inparticular, the influence of extremely rapid thermal cycles and at high temperatureon the physical, metallurgical and mechanical properties of welded materials alwaysrequires a better understanding. In order to produce this work, the multiplicity of knowledge, scientific as well astechnical, to be put in practice has led us to have recourse to a range of authors toshare the task. The disadvantage is of course a certain disparity between the variouschapters, as well as the risk of some repetitions. On the other hand, its richness isderived from this very fact as this work brings together the contributions ofnumerous French specialists well known in their specific field. It presents an entityas complete as possible on the knowledge available today on welding, without ofcourse claiming to be exhaustive (for example, the welding of the plastics is outsideits scope). In a first part of 7 chapters, which deals with metallurgy and mechanics ofwelding, Chapters 1 and 2 present all the processes of welding, from the traditionalprocesses with and without filler, with and without mechanical action, to the recentprocesses with high energy, electron beam and laser. Chapter 3 deals with the wholeof the thermal, metallurgical and mechanical phenomena, which occur in the heataffected zone (HAZ) of the base material. Here the transformation phases with allthe consequences they have on the structures and their properties are presented, aswell as the phenomena of cracking, in particular cold cracking, which is a recurringtheme of this work. Chapter 4 is similar but deals with the question of molten metal in the weld, withother phenomena of cracking that are called into play.
Preface xv The different types of filler products are then dealt with in Chapter 5 dependingon the process used. The progress made in the manufacture of these products inorder to improve the properties of the weld and resistance to cracking is explained. Chapters 6 and 7 illustrate the problems of failure in service of weldedconstructions, the former dealing with resistance to fatigue, with solutions suggestedboth for materials and for the execution of the welds, the latter dealing with brittlefailure, with, after setting out the methods of evaluation of the toughness and theevolution of the harmfulness of defects, proposals relating to the composition of theparent material, the quality of the filler metal and the importance of weldingconditions. The second part, Chapters 8 to 14, focuses on the applications of welding forvarious materials and in various industries. First of all, Chapter 8 is devoted to the welding of thin sheets, both bare andcoated, mainly used in the automotive market with the appropriate processes ofwelding. The importance of new steels with a very low percentage of carbon isunderlined. The subject of Chapter 9 is the welding of steel mechanical components in theautomotive industry, with less traditional processes calling upon a minimum ofmolten metal. The welding of steel structures is the subject of Chapter 10. The steels used andthe techniques of welding with the precautions required in order to avoid defects arepresented. Chapter 11 concerns the welding of pressure vessels. It deals with examples oflarge components such as pressurized water reactors (PWRs) in the French nuclearindustry and analyzes the various processes of welding and coatings used accordingto the parts of the vessel. The majority of the preceding chapters refer to welding carbon and low-alloysteels, so Chapters 12 and 13 are devoted to other types of alloys. First of all, thewelding of stainless steels is presented in detail, and for various families(martensitic, ferritic, austenitic and austeno-ferritic) with the concomitant problemsof cracking and embrittlement, as well as the remedies and advice suggestedaccording to the processes selected. Then, the welding of aluminum alloys is tackledwith the various welding techniques used, the problems encountered and the rules torespect in order to obtain welds of good quality.
xvi Metallurgy and Mechanics of Welding Chapter 14 is devoted to standardization developments in welding dealing withthe general organization of quality and standards for non-destructive testing. We extend our thanks to all those authors who have agreed to contribute to thiswork and especially those who work in the industry and who have been willing intheir free time to contribute to this collection of the know-how and current researchin the different fields of welding. Régis BLONDEAU
Chapter 1 Traditional Welding Processes1.1. Introduction To avoid any misunderstandings, the definitions of the terms which appear inthis text are those proposed in the document entitled “Terms and definitions used inwelding and related techniques” published by the “Publications of AutogeneousWelding and the International Council of the French Language” [COL 96]. It has been specified in the preface to this book that welding makes it possible toreconstitute metallic continuity between the components to be assembled. Thisreconstitution involves the re-establishment of the interatomic metal bonding forceswhich requires at the same time a connection of the nodes of the crystal lattices andthe absence of any foreign body likely to constitute a screen. This chapter will successively cover the physical conditions necessary to createthe metallic bond and the industrial processes which make it possible to establishthis bond.1.2. Conditions to create metallic bonding Creating the metal bond consists, theoretically, of bringing the surfaces to belinked closer so that the surface atoms are at a distance of the order of the internodaldistances of their own crystalline system.Chapter written by Guy MURRY and Dominique KAPLAN.
2 Metallurgy and Mechanics of Welding This operation, which would assume at the beginning that surfaces arechemically clean and in a specular state of polish, is not practically feasible. To mitigate this industrial impossibility, the surfaces to be joined will have to beactivated with a view to eliminating the foreign bodies and elements likely toobstruct the creation of the bond.1.2.1. Activation of surfaces The most effective surface activation is fusion which can simultaneously ensuretheir cleaning. The metallic bond is created by solidification. Different procedurescan be employed: a) the two parts to be assembled undergo a surface fusion and thus contribute tothe formation of a molten metal pool (possibly with the addition of a filler) whichsolidifies without mechanical action; b) the two parts to be assembled undergo a surface fusion but an externalmechanical action expels the molten metal and creates the assembly by placing thesurfaces in contact at the solidus temperature; c) the two parts to be assembled undergo a localized fusion and take part in theformation of a captive molten metal core which during its solidification iscompacted by the action of an external effort of compression. The activation of surfaces can also be obtained by heating without fusion. Ingeneral it is then supplemented by a mechanical action which enables, moreover,cleaning and improvement in contact of the surfaces to be assembled. It is possibleto distinguish between: a) the case where the heating and the cleaning of surfaces to be assembled aresimultaneously carried out by mechanical friction (which implies the assembly ofaxisymmetric parts) and is followed, after stopping the latter, by a crushing(“forging”) by axial compression; and b) the case where the heating is carried out by external heating and the closecontact is ensured by an effort perpendicular to the joint plane. Finally, activation can result from a mechanical action without total heating ofthe parts to be assembled. This mechanical action causes a plasticization of the outerlayer of each surface and generates a very localized heating which finally allows theestablishment of the metallic bond. This process simultaneously requires a relativedisplacement of the surfaces to be assembled, parallel to the mating plane, coupledwith a compressive force perpendicular to this same plane. It is necessary to carry
Traditional Welding Processes 3out a careful surface preparation and/or to make sure that relative displacements ofthe latter cause the rejection of the products which pollute them.1.2.2. Elimination of obstacles to bond creation Obstacles to the creation of the metallic bond can be of various kinds: – geometrical surface irregularities, – pollution of the surface (oxides, grease, moisture, etc.), – chemical elements brought in by the surrounding air. Surface irregularities are likely to disrupt the creation of metallic bonds in all thecases where there is not surface fusion of the parts to be assembled. It will then benecessary to carry out a surface preparation by mechanical means (grinding,machining, etc.). All pollution of surfaces to be assembled will have to be eliminated bymechanical action (sanding, grinding) or by chemical means (solvents, scouring,drying, etc.). It is necessary to neutralize the possible effects of chemical elements brought inby the surrounding air. Welding operations generally being carried out inatmospheric conditions, it is especially oxygen, nitrogen and hydrogen (carried inthe air’s humidity) which can be harmful. Oxygen can react with the elements volatilized by the arc and in this waycontribute to the creation of welding fumes. Furthermore, it can especially dissolvein the molten metal and, during solidification, contribute to the formation of: – metallic oxides which constitute inclusions in solidified metal; – porosities in the molten metal due to the drop in solubility which accompaniescooling and solidification. This formation of porosities can be aggravated by areaction developing with an element contained in the metal and leading to theformation of a gas compound (for example, formation and release of CO during steelwelding without protection against the atmosphere). Protection against oxygen in the air can be ensured by the interposition of aneutral gas, a molten slag or by fixing in the form of oxides by the addition ofoxygen hungry elements (silicon especially). In the vicinity of the molten metal, thesurface of the parent metal raised to a high temperature can also react with oxygenand be covered with oxides, which is a further justification for using protectivemeans, including at the back of the weld.
4 Metallurgy and Mechanics of Welding Nitrogen can dissolve in the molten metal and contribute to: – either the formation of porosities in the molten metal due to the drop insolubility which accompanies cooling and solidification; – or the formation of metal nitrides which, according to the conditions in whichthey appear, constitute inclusions or precipitates more or less hardening andweakening in nature; – or for the part which remains in solid solution, a process of weakening byageing. Protection against nitrogen can be ensured by interposing a neutral gas or amolten slag. Hydrogen dissolves in the molten metal and its concentration can reach highlevels, even reaching saturation if precautions are not taken to limit its presence.Hydrogen, the solubility of which decreases when the temperature drops, can thencontribute to the formation: – of porosities during solidification; – of cracks, in a solid state, when, oversaturated, it gathers in the form of gasmolecules on the structural defects of a not very ductile metal. Protection against hydrogen primarily consists of limiting its introduction intothe molten metal by lowering the atomic or ionic hydrogen content of the plasmaarc. To do this it is necessary to minimize the water content of the surrounding air(no welding in a damp atmosphere), to interpose a gas low in hydrogen between thesurrounding air and the arc, to eliminate compounds supplying water (hydroxides,condensation, greases, basic non-dried coatings, fluxes, etc.) and other sources ofhydrogen (cellulose or rutile coatings and grease).1.2.3. How can we classify the various welding processes? At this stage we are led to adopt a system of grading the welding processesaccording to the modes of action and means of protection against the atmosphere(see Table 1.1).
Traditional Welding Processes 5 Activation Complementary action Protection none imperative fusion compression not essential heating compression possible friction compression none Table 1.1. Classing the welding processes according to modes of action and means of protection against the atmosphere Actually, the various welding processes are above all classified according tomore practical criteria, which are: – the energy source applied: flame, electric arc, plasma, Joule effect, spark,induction, friction, explosion, etc.; – the means of protecting the hot metal: gas or slag.1.3. Industrial welding processes Industrial welding processes are set out here according to the criteria definedabove, namely: – processes utilizing the fusion without mechanical action; – processes utilizing the fusion combined with mechanical action; – processes utilizing heating without fusion but with a mechanical action; – processes utilizing a mechanical action without heating. A classification akin to industrial practices will be presented at the end of thischapter.1.3.1. Processes using local fusion of the parts without mechanical action For welding processes operating without voluntary mechanical action, the localfusion of the parts to be assembled can be described by distinguishing the mode ofheating used and the means of protecting the molten metal against the chemicalaction of the surrounding air. Thus, it is possible to list: – flame or gas welding; – plasma welding;
6 Metallurgy and Mechanics of Welding – arc welding; – vertical electroslag welding; – aluminothermic welding. It should be noted that, in all these processes, the molten metal weld pool iscontained in a crucible formed by the shape of the parts to be assembled adjacent inthe mating plane (sometimes the complete closure of the “crucible” is ensured byspecific tools, e.g. slat, slides, mold). In this way a non-molten section of the parts,in the vicinity of the molten metal, is brought up to temperatures, according to itsdistance from the latter, between the temperature of the solidus of the metal and theinitial temperature of the parts. The fraction of this volume (nearest to the moltenmetal), of which the structure and therefore the properties change because of thisheating, is called the heat affected zone (HAZ).22.214.171.124. Flame welding Figure 1.1. Fusion of parent metals and filler metals obtained with a blowtorch The fusion of the parent metals and the filler is obtained by heating with ablowtorch (Figure 1.1) which enables us, by combustion of a gas (acetylenegenerally, hydrogen, propane) with a comburent (which is generally oxygen), tohave an effective flame (of a fuel rating, with acetylene, about 100 to 300 W/cm2 ona spot of heating [RYK 74], the diameter of which is about 5 to 10 cm). This flame comprises two zones, each with a specific role: – a cone at the immediate exit of the blowtorch nozzle whose surface constitutesthe site of primary combustion (this, if acetylene is used, releases hydrogen andcarbon monoxide). At the tip of the cone the temperature is very high (usingacetylene, it exceeds 3,000°C) and the atmosphere is reducing; – a plume where combustion is completed. According to the adjustment of theconsumption ratio, namely the ratio r = volume of oxygen to volume of acetylene,this plume can be oxidizing, neutral or reducing (and thus carburizing for steels). Inwelding a neutral flame is used corresponding to 1 r 1.2. The adjustment ofblowtorch power is made by regulating the flow of acetylene which is governed by
Traditional Welding Processes 7the nozzle diameter. Four nozzle sizes exist which give acetylene flows rangingfrom 10 by 63 l/h to 1,000 by 4,000 l/h. The flow of oxygen is regulatedaccordingly. This choice of acetylene flow takes account of the metal being welded,its thickness, the type of joint and the position of welding. It is possible to add a filler metal which is generally the same composition as themetal being welded and comes in the form of rods (from 1.6 to 5 mm in diameter). Thus, the blowtorch, from the temperatures reached, allows the fusion of metalsand, by its atmosphere, ensures the molten metal is protected against any chemicalreaction with gases in the surrounding air. However, with metals that are very sensitive to oxidation (aluminum, stainlesssteel, copper alloys) it is necessary to use a flux (spread out over the edges requiringwelding or incorporated with the rod) to eliminate oxides formed on the surface.126.96.36.199. Plasma welding Figure 1.2. Plasma non-transferred arc welding Fusion is carried out by heating using a plasma jet. This plasma is generated bythe passage of a known plasma-producing gas (argon, with the possible addition ofhydrogen or helium) in an electric arc created in the annular space formed between acoaxial nozzle and a refractory electrode (Figure 1.2). Generally, in DC, therefractory electrode is negative to avoid its destruction by the bombardment ofelectrons. The recombination in the jet of ionized species in the arc releases greatenergy and as a result generates a very significant rise in temperature which exceeds
8 Metallurgy and Mechanics of Welding10,000°C. The specific power can vary from 500 to 10,000 W/cm2 on a heating spot[RYK 74] whose diameter varies from a few millimeters to a few centimeters). Aperipheral tube ensures the distribution of an inert gas (generally argon or argonmixture + hydrogen) for the protection of the molten metal. This procedure, called anon-transferred arc or blown arc, is reserved for the assembly of relatively thincomponents. Figure 1.3. Plasma transferred arc welding The transfer of heat and therefore thermal efficiency is improved by striking thearc between the refractory electrode and the parts to be assembled. The arc is thenmaintained by a pilot arc which is created between the nozzle and the refractoryelectrode (Figure 1.3). The name given is plasma transferred arc welding. It is theprocedure most commonly used in welding. It makes the assembly of thickerproducts possible (albeit with a variable limit depending on the nature of the basemetal, but in the order of a centimeter), often by using the keyhole procedure; theplasma jet crosses the joint by pushing the weld pool backwards where solidificationoccurs (the faces to be welded can thus be straight edged). In this way completepenetration is ensured and regularized. The use of a support at the back of the weldis generally not necessary because the molten zone is quite narrow (although thisdoes not obviate the need for gas protection at the back). However, this process isnot suitable for carrying out a filler pass. It is generally employed in flat welding andsometimes in horizontal/vertical welding. A filler can be introduced in the form ofwire. To increase the rate of deposit, it can be beneficial to use the hot-wiretechnique. However, the filler can also be introduced in the form of powder into theshielding gas jet (thus around the plasma jet).
Traditional Welding Processes 9 The synchronized generation of electric power pulses in the arc and in theplasma-producing gas flow makes it possible to weld in a vertical position. Such aprocedure requires computerized control of all the parameters.188.8.131.52. Arc welding The contribution of heat used to form the molten weld pool is assured here by anelectric arc operating in DC or AC. The specific power can vary here from 103 to 105W/cm2 on a heating spot [RYK 74] whose diameter varies from a few millimeters toa few centimeters. It must be possible for the arc to be generated easily and then remain stable. Tofacilitate its generation (which will allow us to avoid resorting to a too high startingvoltage compared to the arc’s voltage in permanent mode) as well as to stabilize it,we have recourse to easily ionizable chemical elements which are introduced intothe plasma arc. These elements can come from the fusible and volatile compoundsincluded in the solid products which will form the slag or from gases applied toprotect the molten metal. In addition, the power source must be adapted so that: – its non-load voltage is high enough to allow arc generation, – its normal operating voltage makes it possible to achieve arc lengthscompatible with the technology employed, – its voltage in the event of the arc’s extinction is sufficient to allow the arc to berestored. The choice of polarity, in either AC or DC, must take account of the differentphenomena which occur at the cathode and the anode. Indeed, electron emissiontakes place at the cathode and all the more so if the cathode is heated to a hightemperature. However, if its heating is partially due to the direct Joule effect and thebombardment by the positive ions, it is above all due to the contribution of heatcoming from the Joule effect which occurs in the cathode’s transition zone. This lastpoint explains why the required current depends on the diameter of the cathode; thegreater it is, the higher the current must be to maintain the cathode at a sufficienttemperature. Electrons bombard the anode and thus cause significant heating, increasedfurther by the Joule effect in the anode’s transition zone. If the arc uses DC, the choice of polarity depends especially on the process andthe metal being welded, given that the anodic zone is heated more than the cathodiczone. The AC current supply makes it possible to alternate the phenomena at the twoends of the arc.
10 Metallurgy and Mechanics of Welding When the filler comes from a consumable electrode, the transfer of this metal inthe arc can be achieved in three different ways according to the electric mode of thearc. At high currents, the transfer takes place by pulverization, i.e. in the form ofsmall droplets forcibly projected by the electric field towards the weld pool. At moderate currents the transfer takes place in the form of large droplets which,with little force applied to them, follow irregular trajectories before falling in themolten metal or, possibly in the form of projections to one side – which is generallya sign of a bad adjustment of the welding parameters. At the lowest currents thetransfer takes place by short-circuit. The magnetodynamic effect is insufficient (thecurrent is too low) to detach the droplet from the surface of the electrode; the dropletgrows bigger to the point that it comes into contact with the molten metal. The short-circuit then generates a current surge which detaches the droplet, which isincorporated in the molten metal. The products that ensure the protection of the molten metal can, according to theprocess, be: – fusible compounds which form a slag floating on top (and are likely to reactchemically with it to refine its composition); – often inert gases (argon, helium or mixtures sometimes with the addition ofhydrogen) with, sometimes, the addition of carbon dioxide (whose decomposition inthe arc will give protective carbon monoxide and oxygen which will be fixed byelements introduced with the filler products). In this context, many processes have been developed that can be classifiedaccording to the conditions in which the arc is struck (between the two parts to beassembled or these components and an electrode) and that can also be distinguishedaccording to the conditions in which the welding products are applied.
Traditional Welding Processes 11 Rotating Figure 1.4. Rotating arc welding on pipesa) The arc is struck between the two parts to be assembledArc welding with pressure created with a magnetic field The arc is struck and moves between surfaces to be joined under the effect of apermanent magnetic field judiciously directed and controlled. After surface fusion,the parts to be joined are forced together (there is thus the formation of a seam). Analternative to this process is applied to tubular structures (Figure 1.4) using two coilswhich surround the tube and create two antagonistic magnetic fields. The resultingfield is radial; it thus causes the rotation of the arc in the mating plane. This isrotating arc welding.Arc welding of studs The arc is formed between the end of the stud and the target zone of the support.After fusion of the stud end and creation of a molten pool on the surface of thesupport where the stud is to be fixed, the stud is plunged in the molten metal andmaintained in position until solidification is complete. The power supply and studdisplacement (contact, withdrawal for striking the arc, maintenance then lowering –Figure 1.5) are controlled automatically. The protection of the molten metal isgenerally ensured by the positioning of a refractory containment ring which ensuresalso the “molding” of the molten metal during its solidification. The power source
12 Metallurgy and Mechanics of Weldingcomes from DC or capacitor discharge; the current intensity of the arc is adjustedaccording to the diameter of the stud.b) The arc is struck between a fusible electrode and the components to be assembled Generally, this procedure allows, with each operation, the deposit of a certainquantity of molten metal, a quantity which varies with the type of process andenergy brought into play. It can prove insufficient to form a sufficient seam sectionbetween thick components; it is then necessary to carry out several operations i.e.several passes. Such a situation often requires an edge preparation to be performed,a preparation which ensures proper weld creation (access for the electrode, type ofassembly, position, penetration, possible prevention of deformations, etc.). Thesepreparations have shapes and dimensions which vary especially according to thenature of the base metal and the process employed. The principal varieties are: – straight edged (Figure 1.6a) for assemblies of limited thickness, possibly withspacing between the edges (distance increasing with the thickness). It may benecessary to carry out a pass on the reverse to ensure penetration but it is alsopossible to use a support at the back; Figure 1.5. Stud arc welding
Traditional Welding Processes 13 – V-shaped chamfer (Figure 1.6b) or Y-shaped (Figure 1.6c) with heel andpossible edge spacing. This type of preparation is not employed for thickcomponents because it gives rise to considerable distortion; – X-shaped (Figure 1.6d) with heel and possibly edge spacing. This type ofpreparation requires access to both sides but limits distortion; – asymmetric U-shaped (Figure 1.6e) or, better symmetric (Figure 1.6f) if thereis access to both sides (with heel and possibly edge spacing). This preparation makesit possible to reduce the quantity of molten metal necessary. Sometimes particular preparations such as half-V shaped, half-U shaped (knownalso as J), K-shaped, etc. are used. The processes which will be described are known as “semi-automatic” if theelectrode or the torch is handled by the welder and “automatic” if the latter ispositioned and guided by automated devices. Figure 1.6. Edge preparations
14 Metallurgy and Mechanics of Welding Figure 1.7. Coated electrode arc weldingCoated electrode arc welding The electrode consists of a metallic core (whose diameter varies from 1 to 10 mmand whose length can be up to 450 mm) which serves as the electrical conductor andsupplies the filler metal, as well as an adhesive coating made up of products whichcontribute to the formation of a protective slag and others that volatilize in the arcplasma to stabilize it and, possibly, of metal particles which help form the moltenweld pool (Figure 1.7). This coating can commonly be: – cellulosic: this creates little slag but its combustion releases CO2 andcontributes to the enrichment of the molten metal caused by dissolved hydrogen; – rutile: the basic component is titanium oxide; it contributes to thedesulphurization of the molten metal; the binding agents used release hydrogen; – basic (electrodes used in steel welding): the basic component is calciumcarbonate; it releases little hydrogen but it is hygroscopic and so requires that theelectrodes be correctly baked (300°C approximately) then protected (by maintainingthem at around 100°C for example) before use. Rutilo-basic mixed coatings (better desulfurization) or rutilo-cellulose (goodpenetration) are also proposed as well as coatings containing metal powders toincrease the quantity of metal added (high-output electrodes) or to introducealloying elements.
Traditional Welding Processes 15 Core fusion slightly precedes that of the coating; it forms a crater which directsthe transfer of the filler towards the molten metal. This transfer takes place in theform of large droplets (cellulosic or basic coatings) or by pulverization (rutilecoatings). In many cases, the arc can be DC in origin (the polarity is then selectedaccording to the nature of the base metal, the coating and the welding position) but itis sometimes possible to use an AC current (in particular for steel welding). Theintensity of the current is selected according to the diameter of the electrode; it isgenerally recommended by the manufacturer. Figure 1.8. Arc welding with powdered flux Welding is in practice possible in all positions, each one requiring particularadjustments and appropriate preparation.Arc welding with powdered flux The electrode is a solid wire (approximately 2 to 10 mm in diameter) whosesupply is guaranteed by an automatic device through a torch equipped with a contacttube ensuring the power supply. Upstream of the torch (compared to the direction ofthe welding process) a nozzle in which the arc will be struck distributes thepowdered flux, part of which will constitute the protective slag, whereas the rest,covering the weld area with a layer of non-molten flux which slows down cooling,will be recovered later on. The arc is not visible, so consequently this imposes aprecise piloting of the torch displacement.
16 Metallurgy and Mechanics of Welding This process (Figure 1.8) makes it possible to weld with high currents and a highoutput. However, in general, dilution is significant, about 2/3 and it increases withthe welding current. The arc is struck using DC when the welding intensity does not exceed 1,000 A;the polarity can be direct (the wire is negative) if deep penetration is required orinverse (the wire is positive) if, on the contrary, a high welding speed and areduction in dilution is desired. With elevated currents it is sometimes easier to useAC, which makes it possible to decrease the effects of magnetic arc blow. The Joule effect along the length of wire electrode, between the contact tube andthe arc, heats the filler metal (all the more depending on length and current) andfacilitates its fusion, thus increasing the quantity of filler metal in the weld pool. Fluxes used are mixtures of mineral compounds (generally silicon manganese orsilico-alumino-calcic compounds) delivered in the form of calibrated pellets. Thetwo principal manufacturing processes give them different properties: – so-called molten fluxes are manufactured from minerals by fusion, molded andthen crushed; they thus have a vitreous and/or crystallized structure and can beporous; – so-called agglomerated fluxes are manufactured starting from natural mineralproducts agglomerated or sintered (with a binder). These fluxes can adsorb or absorbwater and so it is necessary to take precautions to avoid any addition of hydrogen. In general, the manufacturers of welding products combine flux and filler metal.Each combination often makes it possible to confer their own specific properties onthe molten metal. This welding process, due to the method of flux application, enables only flatwelding (and possibly at an angle with a special support). It allows straight edgedbutt welding with edge spacing up to significant thicknesses (depending on the basemetal) but to weld very thick components it requires a preparation which account forthe possibility of making a pass(es) on the reverse side: – no access: V-shaped preparation with heel, spacing and support at the back ortulip-shaped preparation or U-shaped with heel; – access: X-shaped with heel and spacing or K-shaped preparation with heel. Furthermore, welding can be accelerated by associating two (or more) weldingheads each with its own power supply; the electrodes are generally placed in tandemat a distance of about 25 to 35 mm.
Traditional Welding Processes 17 Figure 1.9. MIG-MAG weldingGas shielded arc welding with a solid fusible wire The electrode is a solid wire (from approximately 0.5 to 2.4 mm in diameter)whose supply is ensured by an automatic device through a torch equipped with acontact tube ensuring the connection to the power supply. This torch comprises an annular gas delivery which will ensure the protection ofthe molten metal. This gas can be of two types (Figure 1.9). It can be inert and theprocess is then known as MIG (metal inert gas) welding. It can be argon (pure ormixed with helium) which ensures good arc stability and gives a good penetration,or helium mixed with argon; the proportion of argon must be high enough topreserve arc stability. It can be active and the process is then known as MAG (metalactive gas) welding. In this case it contains oxygen and, more often, CO2 mixed withneutral gases (argon mainly). The presence of oxygen (whether supplied or comingfrom the break up of CO2) brings a certain number of advantages: the arc is morestable, the weld pool more fluid, the transfer by pulverization can be establishedover a broader range of power supply conditions, the chamfers are filled better andvoids less likely. However, the risk of loss of elements transported in the arc leads tothe introduction of elements likely to combine with oxygen into the wire electrode. The power is generally supplied in DC and in inverse polarity (positive wireelectrode) in order to increase the speed of wire fusion and to stabilize the mode oftransfer, in the arc, of the molten metal. Two modes are mainly used: – the transfer by axial pulverization for the welding of thick products but limitedto butt and flat angle welding or gutter welding; – the transfer by short-circuit which involves little energy and allows welding ofthin products and all types of in situ welding.
18 Metallurgy and Mechanics of Welding Certain modern equipment makes it possible to superimpose pulses over thebasic current in order to cause the detachment of the drops at fixed frequency andthus to stabilize their size. It then becomes possible to control their transfer and toregulate their flow whatever the welding current. The term used is pulsed welding. Assemblies are made with all the preparation types already evoked but takingaccount of the need to allow sufficient access for the torch. This access can befacilitated by lengthening the wire electrode between the contact tube and the arc,with a resultant increase in the quantity of metal deposited in consequence of theheating by Joule effect in this length of wire and, generally, reduction in penetration.Welding can be carried out in all positions after adaptation of operationalparameters. Figure 1.10. Cored wire arc weldingCored wire arc welding This process (Figure 1.10) is derived from gas shielded solid wire arc welding bya simple replacement of the solid wire with a flux cored wire (diameter from 1 to 4mm). A cored wire consists of a tubular metal envelope filled with a powder (flux)whose composition and role are comparable with those of the coating on a coatedelectrode. According to the manufacturing process of cored wire, this can be closed(by drawing of a hollow cylindrical wire filled with flux) or formed by pleating orcrimping and thus more or less sealed (but it can again comprise two parallel fillingscontaining flux and a metal filler powder). As the fluxes are hygroscopic and themetal sheath more or less sealed, it is necessary to take the same precautions for useas for coated electrodes. However, cored wires without slag (and thus containing
Traditional Welding Processes 19metal powders) enable us, with an effective gas protection, to appreciably increasethe welding speed and the quantity of metal added. As in MIG or MAG welding, the supply of the wire is guaranteed by anautomatic device through a torch equipped with a contact tube ensuring the powerconnection. This torch makes an annular gas supply possible, which will ensureprotection of the molten metal. This gas is generally reactive (CO2, possibly mixedwith argon). The filled wire being more rigid than solid wire makes it possible to furtherincrease the length of the wire electrode between the contact tube and the arc andthus to facilitate access (it is necessary to avoid over lengthening this distance so asnot to separate the molten metal too much from the shielding gas). Assemblies are made with all the types of preparation already evoked by takingaccount of the improved accessibility given by the increased length of the wireelectrode between the contact tube and the arc. This makes it possible to reduce thechamfer openings. In addition, the good penetration makes it possible to increase theheight of the heels and to decrease the spacing between surfaces to be assembled.Welding is generally carried out on the horizontal and sometimes in other positions,in which case, a small diameter cored wire is used. Cored wires are also offered for welding without a shielding gas. Protection isthen assured by both the slag (of which the limited quantity is not sufficient toensure total protection) and by a dense atmosphere generated by specific productsintroduced into the flux. In addition, the metal sheath of the filled wire containselements likely to decrease the harmful effects of an incomplete protection(deoxidizers and denitrifying agents). Finally the welding parameters are adjusted toreduce the length of the arc. These cored wires make it possible to decrease the sizeof the welding torch, to facilitate access and thus limit the preparation required. Figure 1.11. TIG (tungsten inert gas) welding
20 Metallurgy and Mechanics of Weldingc) The arc is struck between a refractory electrode and the components to beassembled The non-consumable electrode consists of a tungsten tip (Figure 1.11) held in atorch equipped with an annular gas delivery which will ensure the protection ofmolten metal. This gas is neutral: argon (sometimes with the addition of hydrogen –up to approximately 30%) or helium. Argon gives good arc stability but heliumensures better thermal efficiency and thus deeper penetration. These considerationsmean that argon-helium mixtures (about 80% Ar and 20% He) are often used. Thisprocess is most commonly called TIG (tungsten inert gas) welding. It can benecessary, depending on the base metal, to set up a gas protection on the reverse sideusing a gas which can be either identical or different from that supplying the torch(nitrogen-hydrogen). The electrode (0.5 to 10 mm in diameter) can be pure tungsten or tungsten withan addition of zirconium oxide (0.3-0.5%) or thorium (1-2%). These additions makeit possible to increase the electrode emission capacity and thus to improve arcstability and help arc initiation. They also increase the electrode performance andthus the acceptable maximum current. The shape of the electrode point is asignificant parameter of TIG welding. The electrode is often pointed in DC mode,and hemispherical in AC. The power supply is generally DC with direct polarity (negative electrode) so asnot to subject the electrode to electron bombardment. In this way the energy impactis concentrated on the parts to be assembled and at the same time a narrow bead andgood penetration are achieved. The arc can also be established by AC (with asuitable power source) when an electronic bombardment is desired to clean the partsto be assembled. Arc initiation is often assisted using a pilot arc. A filler can be introduced directly into the molten metal pool either in the formof rods or in the form of wire using a mechanized reel, allowing, if necessary, thepre-heating of the wire to improve the deposit rate. Assemblies are produced using all the preparation types already evoked abovetaking account on the one hand of the limitation of the volume of molten metal and,on the other hand, of the need for taking particular care (cleanliness, dimensionalaccuracy especially with regard to the spacing of the parts – it can be useful to set upa support on the reverse side). Welding can be carried out in all positions afteradaptation of the operational parameters. An easier use of the TIG process and an increase in penetration can be obtainedby applying a fine layer of a reactive flux to the surface of the edges to beassembled.
Traditional Welding Processes 21 The composition of this flux (often formed of oxides and/or halides) must beselected according to the nature of the base metal. Figure 1.12. Vertical electroslag weldingVertical electroslag welding This process consists of forming a molten metal bath in a verticalparallelepipedal mold formed by the two sections to be assembled and two water-cooled copper shoes applied to the surface of the two parts (Figure 1.12). Thecontinuous supply of molten metal due to the filler fusion (consumable wireelectrode and possibly fusible wire guide) and the progressive solidification of themolten metal little by little consolidate the two parts. Above the molten weld pool, abath of slag (thickness 40 to 60 mm) ensures its protection. The permanent heatingis due to the Joule effect which develops partly in the electrode but especially in thismolten mineral pool. Welding progresses vertically upwards. It begins with thestriking of an arc between the wire electrode and an appendage which closes thebottom of the mold and on which a welding flux is deposited (which will form theslag). When the volume of molten metal is sufficient, the quantity of flux necessary toconstitute the slag layer is introduced; the arc then ceases. It is generally preferableto set up, in the edge prolongation to be assembled, two blocks of the same
22 Metallurgy and Mechanics of Weldingcomposition as the base metal and of the same thickness. The weld’s end point willbe after the molten metal has reached the level of these blocks so that the shrinkageat the end of solidification does not affect the weld per se (any surplus deposit thuscreated will be removed later on). According to the dimensions of the parts to beassembled, the side shoes can be moved upwards to follow the progression ofwelding. The heat affected zone is wide, because of the very significant heat generation.According to the thickness of the parts to be assembled several wire electrodes canbe used simultaneously. To carry out welds of considerable height, a fusible wireguide plunged in the slag and melting simultaneously the wire electrode(s) can beemployed; this fusible wire guide contributes to the molten metal weld pool. Theterm then employed is vertical electroslag welding with fusible wire guide. Theprocedure generally makes use of AC. This process allows butt welding and welding at an angle (by using adaptedshoes) of work pieces whose thickness is generally not less than 40 mm.Aluminothermic welding In this process the welding is carried out by running a metal in fusion (filler) intoa mold built around the two faces of the parts to be assembled, placed face to face, ata specified distance. These two faces are often pre-heated with a flame via holesprovided in the mold. The molten metal is created on the spot by aluminothermy, i.e.exothermic reaction between oxides (of the metal filler) and powdered aluminum.This operation is carried out in a crucible placed at the top of the mold. As themolten filler is run in, the surface of the parts to be assembled melts, precedingsolidification of the assembly. The protection of the molten metal is ensured by theslag which is formed during the aluminothermic reaction. Afterwards, it is necessaryto remove the mold and grind the assembled parts, so as to eliminate any excessdeposits.1.3.2. Processes using local fusion of components with mechanical action The contribution of heat used to form the molten weld pool is assured here by theJoule effect of a high intensity alternating current which crosses the mating plane. Itis the contact resistance between the two surfaces of the parts to be assembled whichmakes it possible to concentrate fusion in this plane. Several processes have been developed that we can classify according to the fatereserved for the molten metal; containment or expulsion. All require rather heavyand specific equipment.
Traditional Welding Processes 184.108.40.206. Resistance welding with containment of the molten metal This process combines the Joule effect and a mechanical pressure applied to theoutside of the assembly, perpendicular to it and right where the molten metal zoneis. This force has the aim of ensuring a good electrical contact between the parts tobe assembled, thereby confining the molten metal in the zone where it is formed andapplying pressure to it after its solidification in order to improve its compactness byavoiding shrinkage (an operation known as spot forging). Generally the electrodescarrying the current apply this effort. These considerations show that they areoverlapping assemblies of products of limited thickness. The containment of themolten metal within the joint avoids any contact with the air; the problem of itsprotection thus does not arise. The effectiveness of this process is related to the localization of the zone heatedby the Joule effect, which depends on the electric contact resistance between theparts; precautions must be taken so that, on the one hand, other resistances in seriesin the electric circuit are much lower and that, on the other hand, there is nopossibility of the welding current being diverted to one or more parallel circuits. The piloting of the welding current as well as that of the compression force arehandled by automatisms which can: – apply pressure before the passage of the current, to bring the two componentsinto close contact and to ensure the electrical contact, – adjust the current intensity and limit its duration (in general, of a few periods toa few tens of periods i.e. durations which are calculated in tenths of a second), – adjust the pressure during the passage of the current to prevent the surfacesseparating (due to dilation) and the consequent dispersion of the molten metal, – maintain or increase the effort to ensure the compactness of the volume ofmolten metal, – if required, run a reduced current as a post-heating. The electrodes are copper-based alloys. The addition of alloying elements (Cr,Zr, W, Cd, Co, Be, etc.) confers the necessary mechanical performance withoutoverly affecting their electric conductivity and thermal conductivity. Their contactsurface to be welded must be clean and uniform in shape.
24 Metallurgy and Mechanics of Welding Figure 1.13. Resistance spot welding In this way resistance spot welding, projection and roller seam welding can becarried out.Resistance spot welding In this process current supply and load application are carried out by cylindricalelectrodes with tips in the shape of a truncated cone cooled by internal watercirculation. Their contact surface is generally flat or slightly convex. They areinstalled on fixed machines or mobile tools; it is always desirable that the step-downcurrent transformer is placed as close as possible to the welding zone. The volume of molten metal has an ovoid form and is called a spot weld. Thewelding is discontinuous and a seal cannot be guaranteed. The final load applicationgenerally causes an indentation on the two faces of the joint; it is possible to avoidon one of the two faces by replacing the electrode with a copper plate through whichthe welding current passes. Figure 1.14. Projection welding
Traditional Welding Processes 25 It is possible, in certain cases, to carry out two spot welds simultaneously bycoupling two transformers (double spot in series with push-pull assembly), or withonly one transformer (provided that it is possible to control the currents).Resistance projection welding In this welding process (Figure 1.14), the passage of the current is localized byraised areas called projections created on one or both of the assembly surfaces.These bosses are stamped on thin flat sheets and machined in other cases. Thesupply of the current and the load application are applied, generally, using plates;during the heating and fusion the bosses collapse and the mobile plate must reactvery quickly to ensure the close contact of the parts to be assembled. If the powersupply is powerful, it is possible and economic to weld several bossessimultaneously. The wear of the plates and deformation of the components areminimal. The geometry of the projections must be precisely controlled.Roller resistance welding In roller resistance welding (Figure 1.15), the electrodes are replaced by copperor copper alloy discs called rollers. These rollers are driven to ensure theprogression of the components. Of course, they carry the electric current and applythe necessary load. The electric current, in general, is modulated as in spot welding but in arepetitive way and the welding consists of successive spots. It can be: – discontinuous if the successive spots do not overlap. It is possible to stop theroller rotation at each spot and to carry out spot compression, and the result isidentical to that of spot welding. It is also possible to work uninterrupted but in thiscase without forging (the effort applied remains constant), – continuous if the various points overlap, i.e. if the formation of each pointinvolves the partial remelting of the preceding spot. The welding then forms aperfect seal. It is possible, in roller welding, to carry out the seam welding of thin sheets usingthe force applied during welding; the extra thickness is then eradicated. It isnecessary, to achieve this, that the overlap does not exceed one and a half times thethickness and that the sheets to be assembled are gripped very tightly.
26 Metallurgy and Mechanics of Welding Figure 1.15. Roller resistance welding220.127.116.11. Resistance welding with expulsion of the molten metal These processes combine the Joule effect with applied mechanical pressure, afterheating, from outside of the assembly and perpendicular to it, over all its surface.This force has the aim of creating the bond by keeping in close contact the surfacesheated to their solidus temperature. A weld metal bulge is formed at the ends of theassembly, which must then be eliminated. As the heated zone is confined, theproblem of its protection is not relevant. Within this framework two rather differentprocesses are employed.Upset resistance butt welding The effort is applied in two stages: first of all for the cold joining of the parts inorder to allow the passage of the current through the surfaces to be assembled, then,after passage of the current, to ensure the weld bond; an excess, or weld bead, isformed which must be eliminated. The Joule effect is limited to the contact zonebetween the two parts and the heating must bring them up to the forgingtemperature. This process is a large-scale consumer of energy and requires careful preparationof the faces to be assembled (which must be parallel and perpendicular to the effortapplied). Therefore, flash welding is sometimes preferred. An alternative used for the longitudinal closure welding of cold formed sectionsutilizes high frequency (HF) induction heating. The HF current is applied by twocontacts rubbing on the weld edges, above the intended weld, where they are stillseparate.